Lecture 15: Optoelectronic devices: Introduction


 Neil Spencer
 3 years ago
 Views:
Transcription
1 Lecture 15: Optoelectronic devices: Introduction Contents 1 Optical absorption Absorption coefficient Optical recombination 5 3 Recombination and carrier lifetime Photo response time Continuity equation Weak illumination at the surface Optical absorption Opto electronic devices are based on the interaction of light with matter, typically semiconductors. Classic examples of these devices include the solid state semiconductor laser, light emitting diodes, photodetectors, and solar cells. In these devices, light or electromagnetic (EM) radiation is absorbed by the semiconductor and converted into electrical signals (electronhole pairs) or electrical signals are converted to EM radiation (typically in the IRVis UV range). To understand the working of these devices it is essentially to look at light  semiconductor interaction. Consider light of wavelength, λ, incident on a semiconductor with band gap E g. The energy of the radiation E is given by hc. Based on the relation λ between E and E g there can be two conditions. 1. E < E g  semiconductor is transparent, though there could be scattering at the interfaces. 1
2 Figure 1: (a) Energy band diagram for a semiconductor showing the valence and conduction band edges. (b) The density of states monotonically increases from the band edges (c) Occupation probability of electrons and holes in the CB and VB, calculated with respect to the intrinsic Fermi function (d) Product of (b) and (c) gives the concentration of electrons in CB and holes in the VB. Adapted from Physics of semiconductor devices  S.M. Sze. 2. E > E g  semiconductor is opaque and the radiation gets absorbed. Typically, this absorption produces electrons in the conduction band and holes in the valence band. Light absorption occurs for photon energies larger than E g, in direct band gap semiconductors. For indirect band gap semiconductors, absorption is usually small, unless the photon energy is larger than the direct gap value. The electrons and holes that are produced are unstable and lose energy to the lattice, i.e.thermalize, and move to the valence and conduction band edges. This can be understood by looking at the occupation probability (f(e).g(e)) which is maximum close to the band edges, summarized in figure 1. If light of energy E greater than E g is incident on a semiconductor then the excess energy (E E g ) is lost to the lattice vibrations as heat (thermalization). The optical absorption process is summarized in figure 2. Let I 0 be the intensity of the incident radiation. The units of intensity are usually W m 2 or Jm 2 s 1. This is related to the photon flux (Γ ph ) and the energy of the radiation (hυ) by I 0 = Γ ph (hυ) (1) 1.1 Absorption coefficient The absorption of the photons is proportional to the thickness, for one dimensional absorption with the radiation perpendicular to the surface. If I(x) is the intensity of the radiation at some depth x within the semiconductor, 2
3 Figure 2: Optical absorption process in a semiconductor. Photons of energy equal to and greater than the band gap cause excitation of electrons. Higher energy electrons thermalize to the band edges. Adapted from Principles of Electronic Materials  S.O. Kasap. then the change in intensity for an incremental change in distance (δx) is given by δi = α δx I(x) = I 0 exp( αx) (2) This is shown schematically in figure 3. This is called the BeerLambert law where α is the absorption coefficient, with units m 1. According to equation 2 the intensity reduces exponentially as the depth within the semiconductor increases. Given that the energy does not change, elastic scattering, this means that the photon flux reduces with distance. The maximum flux is at the surface. It is possible to define a penetration depth equal to 1 α. At this distance I(x) = I 0 e, i.e. the incident flux reduces by e. The absorption coefficient, α, is a function of the wavelength (energy) of the photon. When the photon energy is less than the band gap, the absorption is really small, while for energies above the band gap, photon absorption creates electronhole pairs. This depends on the density of states distribution in the valence and conduction band, as shown in figure 4. The optical absorption coefficient also depends on whether the semiconductor has a direct or indirect band gap. The dependence of α on photon 3
4 Figure 3: Intensity drop with depth inside a semiconductor, due to absorption. There is an exponential decrease in intensity as depth increases. Adapted from Principles of Electronic Materials  S.O. Kasap. Figure 4: Electronhole pair creation by optical absorption. The concentration is proportional to the number of available states, given by the density of states function. Adapted from Principles of Electronic Materials  S.O. Kasap. 4
5 Figure 5: Absorption coefficient vs. photon energy for Si and GaAs. Si has a gradual rise in α beyond its band gap since it is an indirect band gap semiconductor, while the rise in α is sharper for GaAs (direct E g ). Adapted from Principles of Electronic Materials  S.O. Kasap. energy is compared for Si and GaAs, in figure 5. When hυ is less than E g the absorption is negligible. When hυ is equal to E g in a direct band gap semiconductor absorption takes place from VB edge to CB edge. Since the DOS states at the band edges are small the value of α is also small. But when photon energy increases even slightly above E g (e.g. k B T above E g ), there is a rapid increases in the number of available states and α increases rapidly. This is seen in figure 5 for GaAs where there is rapid increase in α at 1.43 ev, corresponding to the band gap. Beyond E g, the actual shape of the absorption coefficient curve depends on the shape of the DOS. For an indirect band gap semiconductor, like Si, absorption occurs when there is a lattice vibration (phonon) assisting the photon absorption. So the absorption coefficient increases less slowly above E g, compared to GaAs. 2 Optical recombination Optical absorption results in the production of electronhole pairs. These electron  hole pairs then recombine to produce photons. For a direct band gap semiconductor, the photon energy is equal to E g, while for an indirect 5
6 Figure 6: Recombination in GaAs shown using (a) E vs. k diagram (b)a schematic energy band diagram. The transition give rise to photons of energy equal to E g. For GaAs, this photon lies in the infra red region. Adapted from Principles of Electronic Materials  S.O. Kasap. band gap semiconductor recombination is usually mediated by a recombination center. The recombination in GaAs is shown in figure 6. The recombination in Si, mediated by a recombination center, is shown in figure 7. Recombination can also occur through defect states located in the band gap. These are usually localized states. Defect states located close to the band edges (valence or conduction) are called shallow states and aid in optical recombination. On the other hand, defect states located close to the center of the band gap are called deep states and cause indirect recombination with preferential release of heat rather than light. 3 Recombination and carrier lifetime Consider a ntype semiconductor at room temperature with a dopant concentration (N D ) of cm 3. For Si, with n i of cm 3, this gives a hole concentration (p) of cm 3. The electron concentration (n) equals N D since the dopants are fully ionized. This sample is now uniformly illuminated with light (> E g ) to create excess carriers (electrons and holes), as shown in figure 8. Let n = p be the excess carriers. In weak illumination, n n i.e. the excess concentration is negligible compared to the 6
7 Figure 7: Indirect recombination in Si mediated by a recombination center. Since there is a change in electron wavevector, k, this process involves the lattice vibrations in Si, i.e. phonons. Adapted from Principles of Electronic Materials  S.O. Kasap. Figure 8: Weak illumination in Si. This happens when the number of electronhole pairs created is smaller than the dopant concentration. In this scenario only the minority carrier concentration is significantly affected, while changes in majority carrier concentration can be ignored. Adapted from Principles of Electronic Materials  S.O. Kasap. 7
8 Figure 9: Carrier generation (a) equilibrium (b) during illumination and (c) once the light is turned off. After a certain time interval (determined by minority carrier lifetime) the system returns to state (a). Adapted from Principles of Electronic Materials  S.O. Kasap. majority carrier concentration. There is only a significant change in the minority carrier concentration. In the presence of light, with a nonequilibrium carrier concentration, np n 2 i, the law of mass action is not valid. The new electron and hole concentration, under weak illumination, are given by n = N D p = n2 i N d + n N D + p p (3) Consider a particular example, n = p = cm 3. Then, the new electron concentration, per equation 3, is cm 3. This is a change of only 1%. On the other hand, the new hole concentration is cm 3, or a change of approximately %. The conclusion is that weak illumination leads to a drastic increase in minority carrier concentration. When the illumination is turned off, these excess carriers recombine and the original carrier concentration is obtained, as shown in figure 9. The time required for the system to return to equilibrium is given by the minority carrier lifetime, τ h. τ h defines the average time the hole exists in the valence band before the electron from the conduction band recombines with it. Similarly, for a p type semiconductor it is possible to define a minority carrier lifetime for electrons, τ e, to exist in the conduction band before recombination. If G ph is the rate of generation of carriers, then it is possible to write a general equation relating 8
9 Figure 10: (a) Uniform illumination of a nsemiconductor for a fixed time. (b) The minority carrier concentration before, during, and after illumination is plotted. This is a case of weak illumination so that changes in the electron concentration can be ignored. In this example illumination time is orders of magnitude higher than the recombination time. The plot is generated in MATLAB. this to the excess carrier concentration ( p) and the carrier lifetime (τ h ) d p dt = G ph p τ h (4) The first term on the right hand side refers to generation of new carriers and the second terms represents the loss of the new carriers due to recombination. At steady state the rate of change of carrier concentration is zero. This means that the generation rate is equal to the recombination rate. 3.1 Photo response time Consider ndoped Si with dopant concentration of cm 3, that is uniformly illuminated with light for a certain duration, after which it is turned off. The material is at room temperature and the photon flux is cm 3 s 1 and the minority (hole) carrier lifetime is (τ h ) 50 ns. The illumination profile is shown schematically in figure 10(a). When, initially, there is no light, the minority carrier concentration is given by p n0, the equilibrium hole concentration, which is very small compared to N D and n i. For this particular example, p 0 is cm 3. If G ph is the photon flux impinging on the semiconductor, and if the process is 100% efficient, it produces G ph electronhole pairs. Under conditions of weak uniform illumination, the change in electron 9
10 concentration can be neglected, while the hole concentration (i.e. the minority concentration) change is substantial. Let the time when illumination is turned on be set as the origin, i.e. t = 0. Then, by solving equation 4, it is possible to write an expression for the hole concentration as a function of time, using the initial condition that at t = 0, p n = 0. This gives the hole concentration during illumination as [ p n (t) = τ h G ph 1 exp( t ] ) (5) τ ph where τ h is the hole lifetime (minority carrier lifetime). At steady state, rate of change of hole concentration is zero, so that using equation 4, p n = G ph τ h. This is reached after a time t > τ h. After steady state is reached, the illumination is switched off at time t off τ h, as shown in figure 10(a). The excess hole concentration starts to reduce and this can be obtained by solving equation 4 with G ph = 0. This gives p n (t ) = τ h G ph exp( t τ h ) t = t t off (6) Once the light is turned off the excess carrier concentration decreases exponentially towards the original value. The change in hole concentration, as a function of time, is shown in figure 10(b). There is a rapid increase to the equilibrium concentration and then when the light is turned off the value quickly reduces back to equilibrium. This increase and decrease is controlled by the carrier lifetime, τ h. Smaller the value of τ h, faster is the return to p n0, i.e. the equilibrium situation. A similar set of equations and solutions can be written for a ptype semiconductor under weak illumination, where the minority carriers are electrons. The system is controlled by the electron lifetime, τ e. 4 Continuity equation Carrier concentration during uniform illumination is a specific example of a more general case of light illumination on a semiconductor. Typically, illumination occurs at or close to the surface, where excess carriers are generated. As depth increases, the carrier generation also decreases. But excess carriers generated at the surface diffuse into the material due to the presence of a concentration gradient. When an external field is applied the electric field that is setup can also affect carrier motion. This is summarized in figure
11 Figure 11: Illumination at the surface creates excess carriers and there is a diffusion current into the bulk. There is also a drift current due to the applied external field. In this figure, electron drift and diffusion are in opposite directions, while hole drift and diffusion are in the same direction. Adapted from Principles of Electronic Materials  S.O. Kasap. It is possible to write equations for total electron and hole current (J e and J h ), taking both drift and diffusion into account. J e = neµ e E x + ed e dn dx J h = peµ h E x ed h dp dx D e and D h are the diffusion coefficients, which are in turn related to the drift mobilities, µ e and µ h by the Einstein relation D e = D h = k BT µ e µ h e Equation 7 is similar to the Fick s first law of diffusion equation except that there is also a drift term along with the diffusion term. J e and J h are currents at steady state, similar to a steady state flux. Similar, to Fick s second law, which is an example of nonsteady state diffusion, it is possible to write a generalized equation for excess carriers in the case of nonuniform illumination. Consider an elemental volume in a semiconductor, as shown in figure 12. Hole motion is along the positive x direction so that it uniform across the cross section. Within this elemental 11 (7) (8)
12 Figure 12: Derivation of the continuity equation showing various possible processes in a semiconductor. A small elemental volume is considered. The flux through this volume can be due to diffusion and drift current. Under weak illumination changes in majority carrier concentration can be ignored and only generation and recombination of minority carriers need to be considered. Adapted from Principles of Electronic Materials  S.O. Kasap. volume, the net change in hole concentration is due to a change in a flux (due to diffusion or drift), holes lost due to recombination, and holes created by illumination. This can be represented mathematically by a continuity equation. This is written as p n t = 1 e ( J h x ) p n τ h + G ph (9) If there is no flux of holes equation 9 becomes the same as equation 4, uniform illumination. Under steady state conditions with surface illumination, equation 9 becomes 1 e ( J h x ) = p n τ h (10) If we take the electrical field to be small, so that drift current can be ignored, then equation 7 can be used to write the above equation as d 2 p n dx 2 = p n L 2 h (11) where L h is called the diffusion length and is given by D h τ h. 12
13 Figure 13: Weak illumination at the surface creates excess holes that diffuse into the bulk. Adapted from Principles of Electronic Materials  S.O. Kasap. 4.1 Weak illumination at the surface Consider the situation weak illumination at the surface, with negligible absorption at the depth, as shown in figure 13. Light is incident at the surface of the semiconductor creating electronhole pairs. With increase in depth, light intensity decreases (BeerLambert law, equation 2) so that the carrier generation also decreases. The rapidity of this decreases depends on the penetration depth, which is inversely related to the absorption coefficient for that wavelength. To simply this dependence, it is possible to consider a certain depth x 0 within which carrier generation occurs and there is no generation within the bulk of the semiconductor. Ignoring electrical field variation within the semiconductor, the hole concentration for this system can be obtained by solving equation 11. This gives the solution for excess holes, as a function of distance to be p n (x) = p n (0) exp( x L h ) (12) where p n (0) is the excess hole concentration at the surface. This can be calculated from the photon flux, G ph, and also the width of the region where electronhole pairs are generated (x 0 ). p n (0) = x 0 G ph τh D h (13) It is possible to write a similar equation for the excess electron concentration, as a function of depth, by n n (x) = n n (0) exp( x L e ) n n (0) = x 0 G ph τe D e (14) 13
14 Figure 14: (a) Excess concentration and (b) diffusion current as a function of depth for weak surface illumination. There is an electron and hole diffusion current due to movement of carriers to the bulk. In the absence of any external field this diffusion current is balanced by a drift current. Adapted from Principles of Electronic Materials  S.O. Kasap. Taking the ratio of the two terms gives p n (0) n n (0) = De D h (15) For Si, this ratio is higher than 1. This is because diffusion coefficients are directly related to carrier mobilities, given by equation 8, and electron mobilities are higher than hole mobilities in Si. Again, this is because the electron effective mass in Si in the conduction band is smaller than the hole effective mass in the valence band. For weak illumination, the change the bulk concentration due to the excess electrons created can be neglected. The decrease in the hole concentration as we penetrate within the bulk of the semiconductor leads to a hole diffusion current. This is given by J h = ed h dp n (x) dx The electron diffusion current is given by J e = ed e dn n (x) dx = ed h L h p n (0) exp( x L h ) (16) = ed e L e n n (0) exp( x L e ) (17) The excess carriers and the diffusion currents are plotted in figure 14. In an open circuit the total current in the semiconductor is zero. So that J drift,e = J D,h J D,e (18) 14
15 This drift current arises because the diffusion currents due to electrons and holes are different. The magnitude of the drift current increases with depth until the bulk concentrations are reached, as shown in figure 14. Weak illumination at the surface is a particularly useful case for analyzing the effect of light absorption in a semiconductor. Practical situations lead to more complicated applications of the continuity equation. This is important to calculate emitted intensities in light emitting diodes and light absorption and carrier generation in solar cells and photodetectors. 15
Chemistry Instrumental Analysis Lecture 8. Chem 4631
Chemistry 4631 Instrumental Analysis Lecture 8 UV to IR Components of Optical Basic components of spectroscopic instruments: stable source of radiant energy transparent container to hold sample device
More informationCarriers Concentration and Current in Semiconductors
Carriers Concentration and Current in Semiconductors Carrier Transport Two driving forces for carrier transport: electric field and spatial variation of the carrier concentration. Both driving forces lead
More information3.1 Introduction to Semiconductors. Y. Baghzouz ECE Department UNLV
3.1 Introduction to Semiconductors Y. Baghzouz ECE Department UNLV Introduction In this lecture, we will cover the basic aspects of semiconductor materials, and the physical mechanisms which are at the
More informationCarrier Recombination
Notes for ECE606: Spring 013 Carrier Recombination Professor Mark Lundstrom Electrical and Computer Engineering Purdue University, West Lafayette, IN USA lundstro@purdue.edu /19/13 1 carrier recombinationgeneration
More informationET3034TUx Utilization of band gap energy
ET3034TUx  3.3.1  Utilization of band gap energy In the last two weeks we have discussed the working principle of a solar cell and the external parameters that define the performance of a solar cell.
More information3.1 Absorption and Transparency
3.1 Absorption and Transparency 3.1.1 Optical Devices (definitions) 3.1.2 Photon and Semiconductor Interactions 3.1.3 Photon Intensity 3.1.4 Absorption 3.1 Absorption and Transparency Objective 1: Recall
More informationSemiconductor Physics. Lecture 3
Semiconductor Physics Lecture 3 Intrinsic carrier density Intrinsic carrier density Law of mass action Valid also if we add an impurity which either donates extra electrons or holes the number of carriers
More informationSession 5: Solid State Physics. Charge Mobility Drift Diffusion RecombinationGeneration
Session 5: Solid State Physics Charge Mobility Drift Diffusion RecombinationGeneration 1 Outline A B C D E F G H I J 2 Mobile Charge Carriers in Semiconductors Three primary types of carrier action occur
More informationKATIHAL FİZİĞİ MNT510
KATIHAL FİZİĞİ MNT510 YARIİLETKENLER Kaynaklar: Katıhal Fiziği, Prof. Dr. Mustafa Dikici, Seçkin Yayıncılık Katıhal Fiziği, Şakir Aydoğan, Nobel Yayıncılık, Physics for Computer Science Students: With
More informationExcess carriers: extra carriers of values that exist at thermal equilibrium
Ch. 4: Excess carriers In Semiconductors Excess carriers: extra carriers of values that exist at thermal equilibrium Excess carriers can be created by many methods. In this chapter the optical absorption
More informationLecture 7: Extrinsic semiconductors  Fermi level
Lecture 7: Extrinsic semiconductors  Fermi level Contents 1 Dopant materials 1 2 E F in extrinsic semiconductors 5 3 Temperature dependence of carrier concentration 6 3.1 Low temperature regime (T < T
More informationThe German University in Cairo. Faculty of Information Engineering & Technology Semiconductors (Elct 503) Electronics Department Fall 2014
The German University in Cairo th Electronics 5 Semester Faculty of Information Engineering & Technology Semiconductors (Elct 503) Electronics Department Fall 2014 Problem Set 3 1 a) Find the resistivity
More informationReview of Optical Properties of Materials
Review of Optical Properties of Materials Review of optics Absorption in semiconductors: qualitative discussion Derivation of Optical Absorption Coefficient in Direct Semiconductors Photons When dealing
More informationMTLE6120: Advanced Electronic Properties of Materials. Semiconductor pn junction diodes. Reading: Kasap ,
MTLE6120: Advanced Electronic Properties of Materials 1 Semiconductor pn junction diodes Reading: Kasap 6.16.5, 6.96.12 Metalsemiconductor contact potential 2 ptype ntype ptype ntype Same semiconductor
More informationLEC E T C U T R U E R E 17 Photodetectors
LECTURE 17 Photodetectors Topics to be covered Photodetectors PIN photodiode Avalanche Photodiode Photodetectors Principle of the pn junction Photodiode A generic photodiode. Photodetectors Principle
More informationCourse overview. Me: Dr Luke Wilson. The course: Physics and applications of semiconductors. Office: E17 open door policy
Course overview Me: Dr Luke Wilson Office: E17 open door policy email: luke.wilson@sheffield.ac.uk The course: Physics and applications of semiconductors 10 lectures aim is to allow time for at least one
More informationThis is the 15th lecture of this course in which we begin a new topic, Excess Carriers. This topic will be covered in two lectures.
Solid State Devices Dr. S. Karmalkar Department of Electronics and Communication Engineering Indian Institute of Technology, Madras Lecture  15 Excess Carriers This is the 15th lecture of this course
More informationSEMICONDUCTOR PHYSICS REVIEW BONDS,
SEMICONDUCTOR PHYSICS REVIEW BONDS, BANDS, EFFECTIVE MASS, DRIFT, DIFFUSION, GENERATION, RECOMBINATION February 3, 2011 The University of Toledo, Department of Physics and Astronomy SSARE, PVIC Principles
More informationLecture 8. Equations of State, Equilibrium and Einstein Relationships and Generation/Recombination
Lecture 8 Equations of State, Equilibrium and Einstein Relationships and Generation/Recombination Reading: (Cont d) Notes and Anderson 2 sections 3.43.11 Energy Equilibrium Concept Consider a nonuniformly
More informationRecombination: Depletion. Auger, and Tunnelling
Recombination: Depletion Region, Bulk, Radiative, Auger, and Tunnelling Ch 140 Lecture Notes #13 Prepared by David Gleason We assume: Review of Depletion Region Recombination Flat Quantum Fermi Levels
More informationn N D n p = n i p N A
Summary of electron and hole concentration in semiconductors Intrinsic semiconductor: E G n kt i = pi = N e 2 0 Donordoped semiconductor: n N D where N D is the concentration of donor impurity Acceptordoped
More informationDue to the quantum nature of electrons, one energy state can be occupied only by one electron.
In crystalline solids, not all values of the electron energy are possible. The allowed intervals of energy are called allowed bands (shown as blue and chessboard blue). The forbidden intervals are called
More information A free electron in CB "meets" a hole in VB: the excess energy > a photon energy.
5.4. Recombination and Minority Carrier Injection 5.4.1 Direct and Indirect Recombination A free electron in CB "meets" a hole in VB: the excess energy > a photon energy. Energy CB ψ cb (k cb ) ψ vb (k
More informationcollisions of electrons. In semiconductor, in certain temperature ranges the conductivity increases rapidly by increasing temperature
1.9. Temperature Dependence of Semiconductor Conductivity Such dependence is one most important in semiconductor. In metals, Conductivity decreases by increasing temperature due to greater frequency of
More informationLecture 4  Carrier generation and recombination. February 12, 2007
6.720J/3.43J  Integrated Microelectronic Devices  Spring 2007 Lecture 41 Contents: Lecture 4  Carrier generation and recombination 1. G&R mechanisms February 12, 2007 2. Thermal equilibrium: principle
More informationIn this block the two transport mechanisms will be discussed: diffusion and drift.
ET3034TUx  2.3.3 Transport of charge carriers What are the charge carrier transport principles? In this block the two transport mechanisms will be discussed: diffusion and drift. We will discuss that
More informationESE 372 / Spring 2013 / Lecture 5 Metal Oxide Semiconductor Field Effect Transistor
Metal Oxide Semiconductor Field Effect Transistor V G V G 1 Metal Oxide Semiconductor Field Effect Transistor We will need to understand how this current flows through Si What is electric current? 2 Back
More informationSemiconductor Device Physics
1 Semiconductor Device Physics Lecture 3 http://zitompul.wordpress.com 2 0 1 3 Semiconductor Device Physics 2 Three primary types of carrier action occur inside a semiconductor: Drift: charged particle
More informationCarriers Concentration, Current & Hall Effect in Semiconductors. Prof.P. Ravindran, Department of Physics, Central University of Tamil Nadu, India
Carriers Concentration, Current & Hall Effect in Semiconductors 1 Prof.P. Ravindran, Department of Physics, Central University of Tamil Nadu, India http://folk.uio.no/ravi/semi2013 Conductivity Charge
More informationUNIT  IV SEMICONDUCTORS AND MAGNETIC MATERIALS
1. What is intrinsic If a semiconductor is sufficiently pure, then it is known as intrinsic semiconductor. ex:: pure Ge, pure Si 2. Mention the expression for intrinsic carrier concentration of intrinsic
More informationMTLE6120: Advanced Electronic Properties of Materials. Intrinsic and extrinsic semiconductors. Reading: Kasap:
MTLE6120: Advanced Electronic Properties of Materials 1 Intrinsic and extrinsic semiconductors Reading: Kasap: 5.15.6 Band structure and conduction 2 Metals: partially filled band(s) i.e. bands cross
More informationLN 3 IDLE MIND SOLUTIONS
IDLE MIND SOLUTIONS 1. Let us first look in most general terms at the optical properties of solids with band gaps (E g ) of less than 4 ev, semiconductors by definition. The band gap energy (E g ) can
More informationLecture 12. Semiconductor Detectors  Photodetectors
Lecture 12 Semiconductor Detectors  Photodetectors Principle of the pn junction photodiode Absorption coefficient and photodiode materials Properties of semiconductor detectors The pin photodiodes Avalanche
More informationLuminescence Process
Luminescence Process The absorption and the emission are related to each other and they are described by two terms which are complex conjugate of each other in the interaction Hamiltonian (H er ). In an
More informationSemiconductor Physics
Semiconductor Physics Motivation Is it possible that there might be current flowing in a conductor (or a semiconductor) even when there is no potential difference supplied across its ends? Look at the
More informationEngineering 2000 Chapter 8 Semiconductors. ENG2000: R.I. Hornsey Semi: 1
Engineering 2000 Chapter 8 Semiconductors ENG2000: R.I. Hornsey Semi: 1 Overview We need to know the electrical properties of Si To do this, we must also draw on some of the physical properties and we
More informationFall 2014 Nobby Kobayashi (Based on the notes by E.D.H Green and E.L Allen, SJSU) 1.0 Learning Objectives
University of California at Santa Cruz Electrical Engineering Department EE145L: Properties of Materials Laboratory Lab 7: Optical Absorption, Photoluminescence Fall 2014 Nobby Kobayashi (Based on the
More informationUniform excitation: applied field and optical generation. Nonuniform doping/excitation: diffusion, continuity
6.012  Electronic Devices and Circuits Lecture 2  Uniform Excitation; Nonuniform conditions Announcements Review Carrier concentrations in TE given the doping level What happens above and below room
More informationThe 5 basic equations of semiconductor device physics: We will in general be faced with finding 5 quantities:
6.012  Electronic Devices and Circuits Solving the 5 basic equations  2/12/08 Version The 5 basic equations of semiconductor device physics: We will in general be faced with finding 5 quantities: n(x,t),
More informationPhysics of Semiconductor Devices. Unit 2: Revision of Semiconductor Band Theory
Physics of Semiconductor Devices Unit : Revision of Semiconductor Band Theory Unit Revision of Semiconductor Band Theory Contents Introduction... 5 Learning outcomes... 5 The Effective Mass... 6 Electrons
More informationChapter 1 Overview of Semiconductor Materials and Physics
Chapter 1 Overview of Semiconductor Materials and Physics Professor Paul K. Chu Conductivity / Resistivity of Insulators, Semiconductors, and Conductors Semiconductor Elements Period II III IV V VI 2 B
More informationSemiconductor device structures are traditionally divided into homojunction devices
0. Introduction: Semiconductor device structures are traditionally divided into homojunction devices (devices consisting of only one type of semiconductor material) and heterojunction devices (consisting
More informationClassification of Solids
Classification of Solids Classification by conductivity, which is related to the band structure: (Filled bands are shown dark; D(E) = Density of states) Class Electron Density Density of States D(E) Examples
More informationChapter 12: Semiconductors
Chapter 12: Semiconductors Bardeen & Shottky January 30, 2017 Contents 1 Band Structure 4 2 Charge Carrier Density in Intrinsic Semiconductors. 6 3 Doping of Semiconductors 12 4 Carrier Densities in Doped
More informationSolar cells operation
Solar cells operation photovoltaic effect light and dark V characteristics effect of intensity effect of temperature efficiency efficency losses reflection recombination carrier collection and quantum
More informationECE 606 Homework Week 7 Mark Lundstrom Purdue University (revised 2/25/13) e E i! E T
ECE 606 Homework Week 7 Mark Lundstrom Purdue University (revised 2/25/13) 1) Consider an n type semiconductor for which the only states in the bandgap are donor levels (i.e. ( E T = E D ). Begin with
More informationSemiconductor Physics fall 2012 problems
Semiconductor Physics fall 2012 problems 1. An ntype sample of silicon has a uniform density N D = 10 16 atoms cm 3 of arsenic, and a ptype silicon sample has N A = 10 15 atoms cm 3 of boron. For each
More informationIntroduction to Sources: Radiative Processes and Population Inversion in Atoms, Molecules, and Semiconductors Atoms and Molecules
OPTI 500 DEF, Spring 2012, Lecture 2 Introduction to Sources: Radiative Processes and Population Inversion in Atoms, Molecules, and Semiconductors Atoms and Molecules Energy Levels Every atom or molecule
More informationDensity of states for electrons and holes. Distribution function. Conduction and valence bands
Intrinsic Semiconductors In the field of semiconductors electrons and holes are usually referred to as free carriers, or simply carriers, because it is these particles which are responsible for carrying
More informationBasic Semiconductor Physics
6 Basic Semiconductor Physics 6.1 Introduction With this chapter we start with the discussion of some important concepts from semiconductor physics, which are required to understand the operation of solar
More informationEE495/695 Introduction to Semiconductors I. Y. Baghzouz ECE Department UNLV
EE495/695 Introduction to Semiconductors I Y. Baghzouz ECE Department UNLV Introduction Solar cells have always been aligned closely with other electronic devices. We will cover the basic aspects of semiconductor
More informationSemiconductor Devices and Circuits Fall Midterm Exam. Instructor: Dr. Dietmar Knipp, Professor of Electrical Engineering. Name: Mat. Nr.
Semiconductor Devices and Circuits Fall 2003 Midterm Exam Instructor: Dr. Dietmar Knipp, Professor of Electrical Engineering Name: Mat. Nr.: Guidelines: Duration of the Midterm: 1 hour The exam is a closed
More informationSolid State Physics SEMICONDUCTORS  IV. Lecture 25. A.H. Harker. Physics and Astronomy UCL
Solid State Physics SEMICONDUCTORS  IV Lecture 25 A.H. Harker Physics and Astronomy UCL 9.9 Carrier diffusion and recombination Suppose we have a ptype semiconductor, i.e. n h >> n e. (1) Create a local
More informationChapter 4. Photodetectors
Chapter 4 Photodetectors Types of photodetectors: Photoconductos Photovoltaic Photodiodes Avalanche photodiodes (APDs) Resonantcavity photodiodes MSM detectors In telecom we mainly use PINs and APDs.
More information16EC401 BASIC ELECTRONIC DEVICES UNIT I PN JUNCTION DIODE. Energy Band Diagram of Conductor, Insulator and Semiconductor:
16EC401 BASIC ELECTRONIC DEVICES UNIT I PN JUNCTION DIODE Energy bands in Intrinsic and Extrinsic silicon: Energy Band Diagram of Conductor, Insulator and Semiconductor: 1 2 Carrier transport: Any motion
More informationEE 6313 Homework Assignments
EE 6313 Homework Assignments 1. Homework I: Chapter 1: 1.2, 1.5, 1.7, 1.10, 1.12 [Lattice constant only] (Due Sept. 1, 2009). 2. Homework II: Chapter 1, 2: 1.17, 2.1 (a, c) (k = π/a at zone edge), 2.3
More informationpn JUNCTION THE SHOCKLEY MODEL
The pn Junction: The Shockley Model ( S. O. Kasap, 1990001) 1 pn JUNCTION THE SHOCKLEY MODEL Safa Kasap Department of Electrical Engineering University of Saskatchewan Canada Although the hole and its
More informationDirect and Indirect Semiconductor
Direct and Indirect Semiconductor Allowed values of energy can be plotted vs. the propagation constant, k. Since the periodicity of most lattices is different in various direction, the Ek diagram must
More informationLecture 2. Introduction to semiconductors Structures and characteristics in semiconductors
Lecture 2 Introduction to semiconductors Structures and characteristics in semiconductors Semiconductor pn junction Metal Oxide Silicon structure Semiconductor contact Literature Glen F. Knoll, Radiation
More informationThe Electromagnetic Properties of Materials
The Electromagnetic Properties of Materials Electrical conduction Metals Semiconductors Insulators (dielectrics) Superconductors Magnetic materials Ferromagnetic materials Others Photonic Materials (optical)
More informationWhat do we study and do?
What do we study and do? Light comes from electrons transitioning from higher energy to lower energy levels. Waveparticle nature of light Wave nature: refraction, diffraction, interference (labs) Particle
More informationsmal band gap Saturday, April 9, 2011
small band gap upper (conduction) band empty small gap valence band filled 2s 2p 2s 2p hybrid (s+p)band 2p no gap 2s (depend on the crystallographic orientation) extrinsic semiconductor semimetal electron
More informationCharge Carriers in Semiconductor
Charge Carriers in Semiconductor To understand PN junction s IV characteristics, it is important to understand charge carriers behavior in solids, how to modify carrier densities, and different mechanisms
More informationThe photovoltaic effect occurs in semiconductors where there are distinct valence and
How a Photovoltaic Cell Works The photovoltaic effect occurs in semiconductors where there are distinct valence and conduction bands. (There are energies at which electrons can not exist within the solid)
More informationSemiconductor Physical Electronics
Semiconductor Physical Electronics Sheng S. Li Department of Electrical Engineering University of Florida Gainesville, Florida Plenum Press New York and London Contents CHAPTER 1. Classification of Solids
More informationCME 300 Properties of Materials. ANSWERS: Homework 9 November 26, As atoms approach each other in the solid state the quantized energy states:
CME 300 Properties of Materials ANSWERS: Homework 9 November 26, 2011 As atoms approach each other in the solid state the quantized energy states: are split. This splitting is associated with the wave
More informationEECS130 Integrated Circuit Devices
EECS130 Integrated Circuit Devices Professor Ali Javey 8/30/2007 Semiconductor Fundamentals Lecture 2 Read: Chapters 1 and 2 Last Lecture: Energy Band Diagram Conduction band E c E g Band gap E v Valence
More informationPHYS485 Materials Physics
5/11/017 PHYS485 Materials Physics Dr. Gregory W. Clar Manchester University LET S GO ON A (TEK)ADVENTURE! WHAT? TRIP TO A MAKER S SPACE IN FORT WAYNE WHEN? THURSDAY, MAY 11 TH @ 5PM WHERE? TEKVENTURE
More informationECE 250 Electronic Devices 1. Electronic Device Modeling
ECE 250 Electronic Devices 1 ECE 250 Electronic Device Modeling ECE 250 Electronic Devices 2 Introduction to Semiconductor Physics You should really take a semiconductor device physics course. We can only
More informationElectron Energy, E E = 0. Free electron. 3s Band 2p Band Overlapping energy bands. 3p 3s 2p 2s. 2s Band. Electrons. 1s ATOM SOLID.
Electron Energy, E Free electron Vacuum level 3p 3s 2p 2s 2s Band 3s Band 2p Band Overlapping energy bands Electrons E = 0 1s ATOM 1s SOLID In a metal the various energy bands overlap to give a single
More informationWhat are Lasers? Light Amplification by Stimulated Emission of Radiation LASER Light emitted at very narrow wavelength bands (monochromatic) Light
What are Lasers? What are Lasers? Light Amplification by Stimulated Emission of Radiation LASER Light emitted at very narrow wavelength bands (monochromatic) Light emitted in a directed beam Light is coherenent
More informationB12: Semiconductor Devices
B12: Semiconductor Devices Example Sheet 2: Solutions Question 1 To get from eq. (5.70) of the notes to the expression given in the examples sheet, we simply invoke the relations n 0 p 0, n 0 n 0. In this
More informationL5: Surface Recombination, Continuity Equation & Extended Topics tanford University
L5: Surface Recombination, Continuity Equation & Extended Topics EE 216 : Aneesh Nainani 1 Announcements Project Select topic by Jan 29 (Tuesday) 9 topics, maximum 4 students per topic Quiz Thursday (Jan
More informationChalcogenide semiconductor research and applications. Tutorial 2: Thin film characterization. Rafael Jaramillo Massachusetts Institute of Technology
Chalcogenide semiconductor research and applications Tutorial 2: Thin film characterization Rafael Jaramillo Massachusetts Institute of Technology Section 1: Measuring composition August 20, 2017 Jaramillo
More informationQuiz #1 Practice Problem Set
Name: Student Number: ELEC 3908 Physical Electronics Quiz #1 Practice Problem Set? Minutes January 22, 2016  No aids except a nonprogrammable calculator  All questions must be answered  All questions
More informationSheng S. Li. Semiconductor Physical Electronics. Second Edition. With 230 Figures. 4) Springer
Sheng S. Li Semiconductor Physical Electronics Second Edition With 230 Figures 4) Springer Contents Preface 1. Classification of Solids and Crystal Structure 1 1.1 Introduction 1 1.2 The Bravais Lattice
More informationEE 446/646 Photovoltaic Devices I. Y. Baghzouz
EE 446/646 Photovoltaic Devices I Y. Baghzouz What is Photovoltaics? First used in about 1890, the word has two parts: photo, derived from the Greek word for light, volt, relating to electricity pioneer
More informationChapter 5. Semiconductor Laser
Chapter 5 Semiconductor Laser 5.0 Introduction Laser is an acronym for light amplification by stimulated emission of radiation. Albert Einstein in 1917 showed that the process of stimulated emission must
More informationLecture 3 Semiconductor Physics (II) Carrier Transport
Lecture 3 Semiconductor Physics (II) Carrier Transport Thermal Motion Carrier Drift Carrier Diffusion Outline Reading Assignment: Howe and Sodini; Chapter 2, Sect. 2.42.6 6.012 Spring 2009 Lecture 3 1
More informationPHOTOVOLTAICS Fundamentals
PHOTOVOLTAICS Fundamentals PV FUNDAMENTALS Semiconductor basics pn junction Solar cell operation Design of silicon solar cell SEMICONDUCTOR BASICS Allowed energy bands Valence and conduction band Fermi
More informationPhoto Diode Interaction of Light & Atomic Systems Assume Only two possible states of energy: W u and W l Energy levels are infinitesimally sharp Optical transitions occur between u and l Monochromatic
More informationV BI. H. Föll: kiel.de/matwis/amat/semi_en/kap_2/backbone/r2_2_4.html. different electrochemical potentials (i.e.
Consider the the band diagram for a homojunction, formed when two bits of the same type of semicondutor (e.g. Si) are doped p and ntype and then brought into contact. Electrons in the two bits have different
More informationThermionic Current Modeling and Equivalent Circuit of a IIIV MQW PIN Photovoltaic Heterostructure
Thermionic Current Modeling and Equivalent Circuit of a IIIV MQW PIN Photovoltaic Heterostructure ARGYRIOS C. VARONIDES Physics and Electrical Engineering Department University of Scranton 800 Linden
More informationSemiconductor Physics fall 2012 problems
Semiconductor Physics fall 2012 problems 1. An ntype sample of silicon has a uniform density N D = 10 16 atoms cm 3 of arsenic, and a ptype silicon sample has N A = 10 15 atoms cm 3 of boron. For each
More informationWhat are Lasers? Light Amplification by Stimulated Emission of Radiation LASER Light emitted at very narrow wavelength bands (monochromatic) Light
What are Lasers? What are Lasers? Light Amplification by Stimulated Emission of Radiation LASER Light emitted at very narrow wavelength bands (monochromatic) Light emitted in a directed beam Light is coherenent
More informationFebruary 1, 2011 The University of Toledo, Department of Physics and Astronomy SSARE, PVIC
FUNDAMENTAL PROPERTIES OF SOLAR CELLS February 1, 2011 The University of Toledo, Department of Physics and Astronomy SSARE, PVIC Principles and Varieties of Solar Energy (PHYS 4400) and Fundamentals of
More informationNote that it is traditional to draw the diagram for semiconductors rotated 90 degrees, i.e. the version on the right above.
5 Semiconductors The nearly free electron model applies equally in the case where the Fermi level lies within a small band gap (semiconductors), as it does when the Fermi level lies within a band (metal)
More informationSemiconductor Physics and Devices
The pn Junction 1) Charge carriers crossing the junction. 3) Barrier potential Semiconductor Physics and Devices Chapter 8. The pn Junction Diode 2) Formation of positive and negative ions. 4) Formation
More informationBasic Principles of Light Emission in Semiconductors
Basic Principles of Light Emission in Semiconductors Class: Integrated Photonic Devices Time: Fri. 8:00am ~ 11:00am. Classroom: 資電 06 Lecturer: Prof. 李明昌 (MingChang Lee) Model for Light Generation and
More informationChapter 5. Carrier Transport Phenomena
Chapter 5 Carrier Transport Phenomena 1 We now study the effect of external fields (electric field, magnetic field) on semiconducting material 2 Objective Discuss drift and diffusion current densities
More informationLecture 1. OUTLINE Basic Semiconductor Physics. Reading: Chapter 2.1. Semiconductors Intrinsic (undoped) silicon Doping Carrier concentrations
Lecture 1 OUTLINE Basic Semiconductor Physics Semiconductors Intrinsic (undoped) silicon Doping Carrier concentrations Reading: Chapter 2.1 EE105 Fall 2007 Lecture 1, Slide 1 What is a Semiconductor? Low
More informationLecture 2. Introduction to semiconductors Structures and characteristics in semiconductors
Lecture 2 Introduction to semiconductors Structures and characteristics in semiconductors Semiconductor pn junction Metal Oxide Silicon structure Semiconductor contact Literature Glen F. Knoll, Radiation
More informationLaser Diodes. Revised: 3/14/14 14: , Henry Zmuda Set 6a Laser Diodes 1
Laser Diodes Revised: 3/14/14 14:03 2014, Henry Zmuda Set 6a Laser Diodes 1 Semiconductor Lasers The simplest laser of all. 2014, Henry Zmuda Set 6a Laser Diodes 2 Semiconductor Lasers 1. Homojunction
More information1 Name: Student number: DEPARTMENT OF PHYSICS AND PHYSICAL OCEANOGRAPHY MEMORIAL UNIVERSITY OF NEWFOUNDLAND. Fall :0011:00
1 Name: DEPARTMENT OF PHYSICS AND PHYSICAL OCEANOGRAPHY MEMORIAL UNIVERSITY OF NEWFOUNDLAND Final Exam Physics 3000 December 11, 2012 Fall 2012 9:0011:00 INSTRUCTIONS: 1. Answer all seven (7) questions.
More informationPN Junctions. Lecture 7
Lecture 7 PN Junctions Kathy Aidala Applied Physics, G2 Harvard University 10 October, 2002 Wei 1 Active Circuit Elements Why are they desirable? Much greater flexibility in circuit applications. What
More informationOptical properties of semiconductors. Dr. Katarzyna Skorupska
Otical roerties of semiconductors Dr. Katarzyna Skoruska band structure of crystalline solids by solution of Schroedinger equation (one e  aroximation) Solution leads to energy bands searated by an energy
More informationCarrier Action: Motion, Recombination and Generation. What happens after we figure out how many electrons and holes are in the semiconductor?
Carrier Action: Motion, Recombination and Generation. What happens after we figure out how many electrons and holes are in the semiconductor? 1 Carrier Motion I Described by 2 concepts: Conductivity: σ
More informationDiodes. anode. cathode. cutoff. Can be approximated by a piecewiselinearlike characteristic. Lecture 91
Diodes mplest nonlinear circuit element Basic operation sets the foundation for Bipolar Junction Transistors (BJTs) Also present in Field Effect Transistors (FETs) Ideal diode characteristic anode cathode
More informationLecture 9  Carrier Drift and Diffusion (cont.), Carrier Flow. September 24, 2001
6.720J/3.43J  Integrated Microelectronic Devices  Fall 2001 Lecture 91 Lecture 9  Carrier Drift and Diffusion (cont.), Carrier Flow September 24, 2001 Contents: 1. QuasiFermi levels 2. Continuity
More informationChapter 6: LightEmitting Diodes
Chapter 6: LightEmitting Diodes Photoluminescence and electroluminescence Basic transitions Luminescence efficiency Lightemitting diodes Internal quantum efficiency External quantum efficiency Device
More information